Download presentation

Presentation is loading. Please wait.

Published byTess Burkley Modified over 2 years ago

1
Acero 2000 Acero 2000 PHYSICAL METALLURGY AND THERMAL PROCESSING OF STEEL Ernesto Gutierrez-Miravete Rensselaer at Hartford Monterrey, Mexico, Julio, 2000

2
Course Outline 1.- Physical Metallurgy of Steel 2.- Phase Transformations in Steel 3.- Solidification of Steel 4.- Heat Treatment of Steel 5.- Welding and Surface Treatment of Steel 6.- Supplementary Reading

3
1.- Physical Metallurgy of Steel Iron Iron-Carbon Alloys Steels

4
1.1.- Iron Thermodynamic Properties Phases Crystal Structures

5
1.2.- Iron-Carbon Alloys Crystal Structures Phases and Microstructures Thermodynamic Properties Phase Diagram

6
1.3.- Steels Alloying Elements Phase Diagrams Thermodynamic Properties Structural Effects Diffusion Real Surfaces

7
Iron, Iron Alloys and Fe-C system Iron –Medium of first transition series: Ar3d 6 4s2 –Earth Crust contains ~ 4% Fe –Tf =1540 C ; Th ~ 750 C –Useful Phase Transformations (bcc-fcc) –Ferromagnetic below 768 C

8
Iron, Iron Alloys and Fe-C system (contd) Interstitials: –H, B, C, N, O Substitutionals: –Mostly transition series left, right and below of Fe Fe-C system is the basis of steel metallurgy

9
Phases and Phase Diagrams Equilibrium Phases –Ferrite ( : T < 906, : 1401 < T <1540 C) –Austenite ( : 906 C < T < 1401 C) –Liquid ( l : T > 1540 C) –Carbide, Nitride, Oxide Compounds Phase Diagrams –Graphic display of stable phases as function of temperature.

10
Crystalline Structures, Microconstituents and Microstructures Equilibrium Crystal Stuctures –Ferrite (Body Centered Cubic; BCC) –Austenite (Face Centered Cubic; FCC) –Carbides, Nitrides, Oxides (Complex)

11
Crystalline Structures, Microconstituents and Microstructures (contd) Equilibrium Microconstituents –Ferrite –Austenite –Pearlite (Ferrite-Carbide Micro-Composite)

12
Crystalline Structures, Microconstituents and Microstructures (contd) Equilibrium Microstructures –Ferrite (Grains, Allotriomorphs, Widmanstatten Side-Plates) –Austenite (Grains - Twinned) –Pearlite (Ferrite-Carbide Colonies)

13
Crystal Defects Vacancies Nv = C exp(- U/kT) Dislocations -Fe (a/2) Stacking Faults -Fe High SFE -Fe Low SFE ( Twinning)

14
Crystal Defects (contd) Grain Boundaries –Low Angle –High Angle Interstitial and Substitutional Atoms Interphase Interfaces –Coherent –Semi-coherent –Incoherent

15
Crystal Defects (contd) Gibbs-Thompson Equation ln (c(r)/c) = 2 V/r R T Surfaces –Crystalline arrangement –Surface strain –Chemical layering

16
Multilayer Structure of Real Surfaces Steel Decarburized steel Steel-Oxide transition zone Wustite layer Magnetite layer Haematite layer

17
Effects of Alloying Elements Physico-chemical properties Mechanical properties Magnetic properties Corrosion resistant properties

18
Alloying Elements Expanded -field –Open (Ni, Co, Mn, Ru, Rh, Os, Ir, Pt) –Compunds (C, N, Cu, Zn, Au) Contracted -field –Closed (Si, Al, Be, P, Ti, V, Mo, Cr) –Compounds (Ta, Nb, Zr)

19
2.- Phase Transformations in Steel Temperature-Time Charts Mathematical Modeling of Thermal Processing of Steel Phase Transformations during Cooling Phase Transformations during Heating Research Techniques

20
2.1.- Temperature-time Charts Casting and Cooling of Liquid Steel Heat Treating Thermomechanical Processing

21
2.2.- Mathematical Modeling of Thermal Processing of Steel Diffusion Heat Transfer Fluid and Solid Mechanics Electromagnetism Microstructural Evolution

22
2.3.- Phase Transformations during Cooling Solidification Pearlite Formation Ferrite Formation Cementite Formation Bainite Formation Martensite Formation

23
2.4.- Phase Transformations during Heating Recrystallization Austenitization Tempering Melting

24
2.5.- Research Techniques Metallography Microscopy Crystallography Mechanical Testing Thermometry Mathematical Modeling

25
Phase Transformations Continuum Rate Equations: Convection, Difusion of Mass, Energy and Electromagnetic Fields, Kinetics Phase Transformation Kinetics Additional Microconstituents Isothermal and Continuous Cooling Transformation Diagrams

26
Continuum Rate Equations Conservation of Mass (Eqn. of Continuity) Conservation of Momentum (Eqn. of Motion) Conditions of Compatibility Conservation of Energy (Energy Eqn.)

27
Continuum Rate Equations (contd) Conservation of Species (Diffusion Eqn. and/or Convection/Diffusion Eqn.) Maxwells Equations Constitutive Equations Boundary Conditions Arrhenius Rate Equation r = A exp(- E/kT)

28
Phase Transformation Kinetics Diffusive Nucleation-Growth Transformations f = (4/3) S o t I G 3 (t - ) 3 d f = 1 - exp(- a t b ) Displacive Transformations (T < Ms) f = max {1 - exp( - K 0 [Ms - T])} Diffusive-Displacive Transformations

29
Phase Transformation Kinetics (contd) Grain Growth ( d = grain diameter) d/ t = K 1 exp(-Q/k T) d (1 - 1/n) Precipitate Growth/Dissolution (diffusion controlled) ( r = precipitate radius) r/ t = {2 D V c / r R T}{ 1/r m - 1/r}

30
Phase Transformation Kinetics (contd) Precipitate Growth/Dissolution (interface controlled) r/ t = {2 K 2 V c/ R T}{ 1/r m - 1/r} Analytical solution (dilute solution) r 2 - r o 2 = 2 a C D t where C = (ci - ce)/(cp-ce) << 1 and a = 1 + r o /( D t) 1/2

31
Phase Transformation Kinetics (contd) Solute balance at a steady state moving solid-liquid interface - D ( c/ x) = V (c L * - c S *) = V c o (1/k - 1) i.e. c(x) = c o + c o (1/k - 1) exp[ - V x/D] Solid-liquid interface stability condition G < m G c = m V (c L * - c S *)/ D

32
Phase Transformation Kinetics (contd) Dendritic growth (primary spacing) 1 = K 3 /V 1/4 G 1/2 Dendritic growth (secondary spacing) 2 = K 4 t s 1/3 Eutectic growth (interlamellar spacing) e = K 5 V 1/2

33
Non-Equilibrium Microconstituents Martensite –Body Centered Tetragonal; BCT –C-supersaturated Ferrite –Laths, Plates, Needles Bainite –BCC-BCT –Ferrite-Carbide Micro-Composite –Laths, Plates

34
Isothermal Transformation Diagrams T t f=0.1 f=0.9 path 1 path 2 path 3

35
Continuous Cooling Transformation Diagrams T t f=0.1 f=0.9 path 1 path 2 path 3

36
Properties of Individual Microconstituents in Steel High-purity Ferrite (single crystal) –Theoretical yield shear stress ~ 2000 MPa –Actual yield shear stress ~ 10 MPa High-purity Ferrite (polycrystal) –Theoretical yield shear stress ~ 6000 MPa –Actual yield shear stress ~ MPa –Grain size dependence = o +K /d 1/2

37
Properties of Individual Microconstituents in Steel (contd) Pearlite –Yield strength MPa –Tensile strength MPa Bainite –Yield strength MPa –Tensile strength MPa Martensite –Yield strength MPa

38
Steel as a Composite Material Rule of Mixtures = a f a + b f b Empirical relations (low C steel) = 15.4 { (%Mn) (%Si) (%pearlite) + 0.5/d 1/2 }

39
Steel as a Composite Material (contd) Empirical relations (eutectoid steel) = /d 1/2 where d = interlamellar spacing (mm)

40
Strengthening Mechanisms in Steel Solid Solution Strengthening Dispersion Hardening Dislocation Strengthening Grain Boundary Strenghening

41
Thermal Processing Techniques and Thermometry Heating and Cooling –Induction and Resistance Heaters –High Energy Density Beams –Molds –Quenching Baths Thermometry and Dilatometry –Temperature Measurement –Volume Measurement

42
Diffractometry/Quantitative Metallography/Image Analysis Diffractometry –X-Rays –Electrons –Neutrons Microscopy –Optical –Electron –Field Ion

43
Diffractometry/ Quantitative Metallography/Image Analysis (contd) Image Analysis –Image acquisition –Digital processing –Thresholding operations –Mathematical morphology operations –Measurements

44
Mechanical Testing Hardness test Tensile test Creep test Fracture test Fatigue test

45
Mathematical Modeling and Computer Simulation Hardware –PC –Workstations –Supercomputers Software –Custom -made –Research –Commercial

46
Reading Verhoeven et al, JOM, Sept 1998 Sundman & Agren, MRS Bull, Apr 1999

47
3.- Thermal Processing of Liquid Steel Liquid-Solid Transformations Microstructure Formation during Solidification Macrostructure Formation during Solidification 3.4.-Mathematical Modeling of Steel Solidification

48
3.1.- Liquid-Solid Transformations Melting and Solidification of Pure Iron Solidification of Liquid Steel to Primary Delta-Ferrite Solidification of Liquid Steel to Primary Austenite Melting of Alloy Additions in Liquid Steel

49
3.2.- Microstructure Formation during Solidification Nucleation of Crystals Dendritic Growth The Peritectic Transformation during Steel Solidification Microsegregation

50
3.3.- Macrostructure Formation during Solidification Formation and Evolution of the Mushy Zone during Solidification of Steel Solute Transport and Settling/Floating of Crystals in the Melt Macrosegregation Contraction during Solidification Stresses from Solidification

51
3.4.-Mathematical Modeling of Steel Solidification Heat Transfer Solute Transport Microstructural Evolution Stress Generation

52
Reading Vanaparthy & Srinivasan, Mod. & Sim. in MSE, Vol. 6, 1998 Schwerdtfeger at al, Met & Matls Trans B, Oct 1998

53
4.- Heat Treating of Steel Hardenability Austenitizing Annealing Quenching Tempering Mathematical Modeling

54
4.1.- Hardenability Concept of Hardenability Physical Foundation of Hardenability Measurement of Hardenability Influence of Hardenability on Structure and Properties

55
4.2.- Austenitizing Nucleation and Growth of Austenite during Austenitization Dissolution of Carbides during Austenitization Austenite Grain Growth during Austenitization

56
4.3.- Annealing Phase Transformations during Isothermal Holding Nucleation and Growth of Ferrite Nucleation and Growth of Pearlite Nucleation and Growth of Cementite

57
4.4.- Quenching Phase Transformations during Continuous Cooling Nucleation and Growth of Bainite The Martensitic Transformation Formation of Composite Microstructures containing Multiple Microconstituents Dimensional Changes

58
4.5.- Tempering Precipitation and Growth of Carbides during Heating Transformation of Retained Austenite during Heating Change of Physical Properties during Tempering Dimensional Changes

59
4.6.- Mathematical Modeling of Heat Treatment of Steel Heat Transfer Solute Transport Microstructure Evolution Stress Generation

60
Reading Homberg, Acta Mater. Vol. 44, 1996 Inoue & Arimoto, J. Matls Eng. & Perf., Feb 1997 Archambault et al, J. Matls Eng. & Perf., Feb 1997

61
5.- Welding and Surface Treatment of Steel Welding of Steel Case Hardening of Steel Surface Hardening by Rapid Heating and Cooling

62
5.1.- Welding of Steel Welding Process Weld Microstructure and Properties Mathematical Modeling

63
5.2.- Case Hardening of Steel Case Hardening Processes Solute Diffusion from the Surface of Steel Decarburization of Steel on Heating Nitriding Mathematical Modeling

64
5.3.- Surface Hardening by Rapid Heating and Cooling Diffusion of Time-Varying Electromagnetic Fields into Steel Surface Heating by Eddy Currents Surface Heating by Focused Beams Phase Transformations during Rapid Surface Heating Mathematical Modeling

65
Reading Mundra et al, Weld. J. WRS, Apr 1997 Bhadeshia, 1999 Mittemeijer & Somers, Surf. Eng, Vol. 13, 1997 Fuhrmann & Homberg, 1999

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google